Automotive Catalysts: Performance,
Characterization and Development
Nelcy Della Santina Mohallem,
Marcelo Machado Viana and Ronald A. Silva
Universidade Federal de Minas Gerais
Nowadays, automotive catalysts have been used to reduce atmospheric emissions, due to
significant parcels of the global emissions of pollutants agents provoked by vehicles.
Automotive exhaust catalysts were introduced in the 70’s decade, because some countries
established restricting laws related to emissions of carbon monoxide (CO), nitrogen oxides
(NOx) and hydrocarbons (HC) by the engines. These products generated by the combustion
process are extremely harmful to health and the environment (Massad et al, 1985). For
example, CO combined with hemoglobin in the bloodstream promotes the reduction of
oxygen-active sites that provokes asphyxia. Nitrogen dioxide (NO2) contributes to
photochemical smog and acid rain, and is irritating to the eyes, skin and respiratory system.
Nitrogen monoxide (NO) is toxic by inhalation and irritating to the eyes and skin. Polycyclic
aromatic hydrocarbons (PAHS) have been identified as carcinogenic compounds. Other
combustion products are: ash, formed mainly by particulate residues of components of the
lubricating oil, and soot, combustible matter in the exhaust gas (smoke). Automotive
catalytic converters have been developed precisely to make these products less toxic
(Morterra et al, 1995; Ismagilov et al, 1998).
The development of catalysts only was possible with the improvement in automotive
engines as the replacement of carburetion system for electronic injection and introduction of
the catalyst in the exhaust systems (Kaspar et al, 2003).
The catalysts of three ways (TWC –Three-Way Catalyst) are advanced systems of emission
treatment of gasoline vehicles that reduce significantly the emissions of carbon monoxide
(CO), hydrocarbons (HC) and nitrogen oxides (NOx) in atmosphere (Collins & Twigg 2007).
Nevertheless, there is a steady increase in world production of vehicles powered by gasoline
and by other types of fuel such as alcohol, gas and mix of fuel, leading to constant research
in order to improve the catalysts already known and to develop new models (Mizukami et
al, 1991; Silva et al, 2009 & Sideris, 1997).
Automotive catalysts are generally available in the form of monolith ceramic as cordierite and
zeolites or metal substrate. The catalyst substrates more used are composed of magnesium
cordierite (2MgO.2A12O3.5SiO2) with a honeycomb structure, which provides a high geometric
surface area, coated with γ-alumina (catalyst wash-coat). This wash-coat is designed to
increase the specific surface area and is the support for precious metals, mainly platinum (Pt),
palladium (Pd) and rhodium (Rh), which promotes the catalytic reduction and oxidation of
New Trends and Developments in Automotive Industry
pollutants gases to more harmless ones, like carbon dioxide, water and nitrogen molecular.
Cerium and zirconium oxides are used in the coating by their oxygen storage capability to
improve catalytic efficiency. (Angelidis & Sklavounos, 1995). A variety of other additives also
are used to stabilize the alumina wash-coat at high temperatures (operational temperature).
Figure 1 illustrates the operation of a three-way catalyst. This catalyst transforms the toxic gas
CO in CO2, which although not so toxic contributes to the increase in greenhouse effect.
Fig. 1. Schematic illustration of the TWC operation.
Fig. 2. (a) Catalyst module, (b) new catalyst (c) poisoned catalyst (d) samples of poisoned
The catalyst can be deactivated by chemical, mechanical or thermal phenomena after some
time of operation, depending on the composition of the used fuel and lubricants, and of the
vehicle adjustment. The chemical deactivation can be promoted by poisoning due to the
Automotive Catalysts: Performance, Characterization and Development
chemisorptions of compounds on the surface of the catalyst; and due to chemical reactions
that produce volatile compounds or inactive phases. The thermal deactivation occurs due to
the sintering process and active metal diffusion. The mechanical deactivation is due to the
deposition of particles from the gas phase onto the pores and catalyst surface, and effects of
abrasion caused by mechanical crushing of the catalyst.
Figure 2a shows a typical catalyst module formed by a metal housing containing the
catalyst. Figure 2b shows a new catalyst and the visual effect of deactivation in a poisoned
catalyst is shown in Figure 2c and 2d. The amount of soot deposited in an used catalyst
depends of the fuel quality, since gasoline contains some amount of contaminants such as
sulfur, and oxygen and nitrogen compounds. A new catalyst sample is shown in Figure 3a
and 3b, and Figure 3c shows the clogging of the honeycomb structure caused by the
poisoning of the catalyst.
Fig. 3. (a) Photography of a catalyst sample, (b) SEM micrograph of a honeycomb structure,
(c) clogging of the honeycomb structure caused by the catalyst poisoning.
Beyond the vehicles powered by gasoline, there has been a move for the utilization of other
types of vehicles that have been developed to use different fuels that produce less CO2,
which cause the greenhouse effect. These fuels are the alcohol, renewable bio-fuel derived
by sugar-cane or corn, gases such as liquefied petroleum gas (LPG) and compressed natural
gas (CNG), or mix of fuels as the used in flex-fuel technology. These alternative fuels have a
lower carbon to hydrogen ratio than gasoline, producing less CO2 per travelled distance,
and reduce the needed of fossil fuel consumption (Cohn, 2005).
New Trends and Developments in Automotive Industry
Some technologies have been developed, adapting the engine for the mixtures of fuels like
gasoline and ethanol with predetermined composition. Moreover, there are the new flex-fuel
technology that is related to the flexibility of choice of the car fuel, where is possible to use
only hydrated alcohol or gasoline, or a mixture of these fuels in any concentration (Delgado et
al, 2007). The people can buy the cheapest fuel, whose prices depend on the economic
moment. The flex-fuel technology is based on sensors that detect the concentration of the
mixture of gasoline and hydrated alcohol, and in the subsequent automatic adjustment of the
engine. The addition of ethanol in gasoline decreases the concentration of CO emissions,
making this process a very interesting technology. Some countries are planning to employ this
technology, since about 85% of the cars produced in Brazil are equipped with this technology.
All of these factors impact the design of TWC, since its geometric surface area until the
alumina thin film formulations. It would be necessary a corresponding catalyst for each type
of used fuel, leading in consideration the type of chemical reaction that occurs in the engine.
But in the reality the catalysts of these new vehicles have been adapted without rigorous
criteria, and they are adjusted according to need (Silva, 2008).
Other factors that influenced the development of TWCs were the economics ones, mainly
the related to the prices of the platinum group metal and of the fuels. The constant increase
and instability in the gasoline price led to the development of more economic engines that
also need different design of catalyst. In this sense, various types of substrate as zeolites or
metallic have been tested and/or used (Collins & Twigg 2007).
Actually, recycling and regeneration of catalysts are common practices. Regeneration
consists in a controlled oxidation at high temperature to eliminate soot and convert sulfides
to oxides. After this process, some catalysts also require additional treatments to recover the
full activity. Non-regenerable catalysts have to be recycled for metals recuperation. This can
be performed either by hydrometallurgy or pyrometallurgy (Angelidis et al, 1995; Silva,
2008; Dufresne, 2007 & Hirokazu, 1999).
In this chapter, textural, morphological and structural characteristics of selected new and
used catalysts, analyzed by gas adsorption, pycnometry, X-ray diffractometry, thermal
analyses and scanning electron microscopy, are shown. EDS and WDS electronic
microprobe were used to detect the composition of the catalysts and their contaminants.
Subsequently, we discuss the textural and morphological changes of automotive catalyst by
effect of high temperatures, which lead to its deactivation. New commercial automotive
catalysts were thermally treated at various temperatures. Micrographies and adsorption-
desorption isotherms were used to verify the changes in the catalyst characteristics with
thermal treatments. Finally, problems about gas emission and the soot present in exhaust
gas are discussed, beyond some aspects about reuse and recycling are considered. Some
solutions about this theme are shown.
2. Textural, morphological and structural characteristics of new and used
Some new and used automotive catalysts of vehicles powered by gasoline, by alcohol, and
by flex fuel, of diverse suppliers, have been analyzed.
The samples have been analyzed by X-ray diffractometry (Rigaku, Geigerflex 3034) with
CuKα radiation, 40kV and 30mA, time constant of 0.5s and crystal graphite monochromator
to identify the phases present (metals and transition metal oxides).